Environ Eng Res > Volume 27(3); 2022 > Article
Choi: Assessment of sulfonation in lignocellulosic derived material for adsorption of methylene blue

### 1. Introduction

Dyeing wastewater discharging facilities in Korea account for only 3.6% of all wastewater discharging facilities, but dyeing wastewater discharge amounts to 22.2% of the total wastewater discharge [1]. Moreover, the load of organic matter discharged from dyeing wastewater reaches 24.3% of the total, and dyeing wastewater is classified as a representative polluted industry in terms of wastewater generation and characteristics of wastewater [1, 2]. Most of the dyes have a complex and stable structure such as an aromatic structure, so it is difficult to decompose by chemical, physical and biological treatment [3]. Therefore, when these dyes are discharged without treatment, not only causes aesthetic problems due to chromaticity, but also the dye interferes with the penetration of sunlight into the water surface, thereby inhibiting photochemical and biological activities of aquatic plants. In addition, dyes pose a potential threat to the assimilation of organisms as they have the potential to pollute groundwater.
Currently, there are several methods of treating dye wastewater such as ozone oxidation treatment, coagulation treatment, advanced oxidation (AOP), and biological treatment etc. The agglomeration process is effective for removing insoluble dyes such as disperse dyes, but is not effective for soluble dyes, has a large amount of sludge, and it is difficult to completely remove chromaticity in water [4, 5]. In the case of ozone treatment, it is effective to remove almost all dyes except for disperse dyes, but ozone has a short half-life and has an economic problem that requires a high cost because ozone must be continuously supplied [1]. Most of the known dye removal processes have a low removal efficiency compared to the operating cost, and particularly removal efficiency for low concentration of dye is very low [5, 6]. On the other hand, the adsorption method is known to be suitable for the removal of dye wastewater because it is simpler to operate than other processes and the cost to enter the process is low [7, 8]. Therefore, studies on removing various dyes using activated carbon have been conducted by many researchers. Activated carbon, which has been widely used as an adsorbent so far, is useful for removing various contaminants because of its relatively large specific surface area and porosity [810]. Recently, biomaterials containing lignocellulosic, for example wheat straw, rice hull, daily palm leaves, tea waste and cashew nut shell, etc., are used to adsorb dyeing wastewater and heavy metals. Many researchers conducted heavy metal removal experiments using unmodified natural ligno-cellulosic biomaterials, and reported many positive results [4, 7, 8, 11]. However, the application of unmodified lignocellulose has significant disadvantages such as low adsorption capacity in aqueous solution and high release of soluble organic compounds [5, 12]. Accordingly, in recent years, there is an increasing tendency to modify lignocellulose-based biomaterials in order to improve the removal efficiency of heavy metals, remove soluble organic compounds, and remove dyes in aqueous solutions. Agricultural waste contains large amounts of lignocellulose [7]. Lignocellulose is a type of complex cellulose, a combination of cellulose, hemicellulose, and lignin, and is one of the most abundant biomass on the planet as a major structural component of woody/non-woody plants [13]. However, currently only about 5% of lignocellulose is used [10].
Lignocellulose has a three-dimensional aromatic structure and, when modified, has high reactivity, so a lot of interest has been focused on lignocellulose-based adsorbents [11, 12]. There are typically physical and chemical transformations in the modification method of lignocellulose. The physical modification is generally simple and inexpensive, but it is not widely used because of its low efficiency [4, 13]. On the other hand, chemical modification has the advantage of being simple and highly efficient. In particular, several researchers have reported that sulfonation increases the adsorption efficiency of cationic heavy metals among chemical methods that can modify lignocellulose [14]. This is because pretreatment of lignocellulose using sulfonation leads to an increase in the negative charge, surface area and porosity of the biomass surface [10, 12]. Similarly, Elangovan et al. [15] reported that pretreatment of mangrove leaves and water lily leaves with sulfuric acid substantially improved the Cr(VI) adsorption capacity. In particular, CS is lignocellulose-based agricultural waste, which can be easily available material, and is very useful as a bio-adsorbent because of its high porosity. Therefore, this study attempted to sulfonate lignocellulose-based cornstalk to modify the surface with negative charges, and to use this to adsorb and remove methylene blue (MB), which is the most widely used cationic dye, from aqueous solution.

### 2.1. Materials

#### 2.1.1. Sulfonation of cornstalks

Corn stalk (CS) was collected from a farmhouse in Gangneung, Korea. The CS was washed with tap water and then rinsed with distilled water to remove contaminants. The washed CS was cut into small pieces and dried in an oven at 85°C for 24 h to completely evaporate moisture. The dried CS was pulverized in a ball mill at 120 rpm for 1 h, separated into 40–60 mesh (0.25–0.4 mm) using an automatic sieve, and stored in a desiccator for use in experiments. A 20 g of CS powder was added to 60 mL of ethyl alcohol cooled to −10°C, mixed well, added to 200 mL of cooled sulfuric acid, and heated not to exceed to 10°C using a reaction device (Yhana (Model SS-200, 50W)). A sulfonation of cornstalk was performed while stirring at 100–150 rpm for 2 d. After that, it was left at room temperature for 2 to 3 h to induce the reaction to occur completely, then washed several times with distilled water until neutral, and dried for 48 h in a dryer. The completed sulfonated corn stalk (SCS) were stored in a desiccator for use in experiments.

MB (3,7-bis(Dimethylamino)-phenothiazin-5-ium chloride) used in the experiment is a basic cationic dye with the widest industrial application range among organic wastes and has a molecular weight of 319.85 g/mol. MB (C16H18N3SCI) is a heterocyclic aromatic chemical compound that exists in a very stable structure in aqueous solution, and when dissolved in a solvent, it is ionized to form C16H18N3S+ and Cl. It has a dark blue green color at room temperature, and exists in the form of three water molecules bound per molecule. MB was used by diluting the product of Tera Pharmaceuticals Inc, Buena Park, USA.

### 2.2. Experimental Design

In the MB adsorption experiment using SCS, a stock solution of 1,000 mg/L was prepared and the concentration of the solution required for the experiment was diluted and used. The experiment was carried out in the form of batch-test. Various amounts (0–20 g/L) of SCS were added to 1 L of dyeing water according to the experimental plan, stirred at 120 rpm, and then sampled at a predetermined time (0, 10, 20, 30, 60, 120 and 240 min). To determine the effect of pH on adsorption efficiency, the pH was adjusted to 2–10 using HCl and NaOH. The influence on the temperature was controlled in the range of 10°C to 30°C, and the parameters were changed, and the sample was taken at a predetermined time while stirring at 120 rpm in a shaking incubator.
Adsorption kinetic studies were conducted various contact time (0–480 min) with different concentration of MB (Co: 20–1,000 mg/L), where the MB concentration was determined using a spectrophotometer (Shimadzu, MINI-1240). Equilibrium isothermal studies were determined at 303K by using different MB concentration (20–1,000 mg/L), constant SCS dosage (1 g/L) and pH 7 ± 0.3 for MB solution. Similar procedure was adopted at the temperature 298–323K, where the other reaction parameters were held constant to study the thermodynamic parameters. For the adsorption kinetics, SCS was mixed with various concentration of MB and then shaken until equilibrium was sufficiently reached. Isothermal adsorption were analyzed using Langmuir, Freundlich and Temkin, and adsorption kinetics were interpreted using Pseudo-first-order, Pseudo-second-order and intraparticle diffusion. Thermodynamic analysis was performed using Gibbs’ free energy.

### 2.3. Analysis Methods

Qualitative and quantitative analysis of inorganic components contained in SCS was analyzed using X-ray diffraction (XRD, XRF-1500, Shimadzu, Japan). The specific surface area, pore volume and average pore diameter of SCS were analyzed using a Brunauer-Emmett-Teller (BET) specific surface measuring machine (Model ASAP, 2020), and the molecular structure and composition of the surface functional groups were analyzed using Fourier-transform infrared spectroscopy (FT-IR, Jasco, FT-IR 4100). The size of the SCS particles was measured using a particle size analyzer (Laser Diffraction Master class 3&4, Malvern, England), and the amount of SCS was measured with an electronic balance (XP26, Mettler Toledo, Swiss). The pH and temperature were measured using a pH meter (SevenGO pro, Mettler Toledo). The collected sample was measured using a UV-vis spectrophotometer (Shimadzu, MINI-1240) at 664 nm, which is the maximum absorption wavelength of MB, and the adsorption amount was calculated using Eq. (1).
##### (1)
$qt=(C0-Ct)VM$
Where C0 is the initial concentration (mg/L), Ct is the concentration at time t, V is the volume of MB solution (L), and M is the amount of SCS (g). The pHpzc was analyzed according to the method reported in a previously published study [16]. All experiments were repeated five times and the average value was used as the experimental result. In order to experiment with one parameter, the other parameter was fixed.
To measure the ion exchange capacity (IEC), chemically treated SCS should be hydrogenated. Generally, a conventional acid–base titration method is used to determine the IEC [17]. The IEC was calculated according to the general Eq. (2).
##### (2)
$IEC (meq/g)=VNaOHNNaOH-VHClNHClWeight of dried sample$
where, VHCl was the volume of HCl entered during quantification in mL, VNaOH was the volume of NaOH used, and NHCl and NNaOH is the normal concentration of HCl and NaOH used, respectively. Resin weight refers to the total weight and 0.2 g of ion exchange resin was obtained by measuring the weight of the resin dried at 110°C for one day.
To select appropriate kinetic and isotherm models for MB adsorption process, Chi-squre (χ2) was calaulated using Eq. (3).
##### (3)
$χ2=Σi=1n(qe,exp-qe,cal)2qe,cal$
where qe,exp and qe,cal are equilibrium adsorption capacity obtained from experiments and models, respectively.

### 3.1. Charateristic of SCS

#### 3.1.1. Physical property

The results of component analysis of CS and SCS are summarized in Table 1. The major constituents of CS and SCS were carbon and oxygen, and in addition they contained small amounts of hydrogen and nitrogen. After sulfonation of CS, the content of oxygen increased and the content of carbon decreased. This may be due to the release of volatiles during the sulfonation process, and the relatively high oxygen content is believed to be due to the high level of chemical active agent used (H2SO4; 95–98%). As the H/C ratio approaches 1, the aromaticity of the bio-adsorbent increases, and when the O/C ratio is high, the anionic properties of the bio-adsorbent are strengthened due to the increase of the carboxylate group in the bio-adsorbent, thereby increasing the ability to adsorb cationic substances [1, 5]. After sulfonation the H/C ratio improved from 0.04 to 0.14, and the O/C ratio increased from 0.65 to 1.27, indicating that the carboxyl group inside the SCS adsorbent increased.
The BET surface area (24.13 m2/g) of SCS increased by about 2.9-fold that of CS, and this increased specific surface area was thought to be due to the high concentration of H2SO4 that enhanced the pore volume and surface area. It was observed by previous studies that biomass results in a high specific surface area when treated with concentrated H2SO4 [18, 19]. It is difficult to establish the relationship of the interaction with the adsorption capacity with only the surface area of the adsorbent because there are many other factors that contribute to the efficiency of the adsorption process. However, many researchers emphasized that the adsorption of MB affects the surface acidity of carbon by various surface functional groups such as phenol and carboxyl groups due to the influence of electrostatic interactions with the adsorbent. It was confirmed by several researchers that such surface acidity affects the adsorption efficiency of MB [6, 12, 2022].

#### 3.1.2. pHpzc

The pHpzc (point of zero charge) is the pH at which the net charge on the surface of the adsorbent becomes zero [25]. The pHpzc is important because the adsorption of some substances depends on the pH of the aqueous solution, and the pzc value is determined by the properties of the adsorbent [1]. From the point of view of the adsorbent, if the pH is lower than the pzc value, the surface charge of the adsorbent becomes positive and anions may be adsorbed. On the contrary, if the pH is higher than the pzc value, the surface charge becomes negative, so that cations may be adsorbed. To find the surface charge of SCS, the experiment was conducted by adjusting the pH to 3–10, and the results are shown in Fig. 1. The ΔpH is the value obtained by subtracting the initial pH from the final pH. The pHpzc of SCS was found to be 5.3, and it was confirmed that there is an acidic functional group on the SCS surface. The negative surface charge of SCS can be found in a pH environment above pHpzc favoring the adsorption of MB cations. In general, the adsorption of MB may be due to the presence of OH, COO-, and SO3 groups on the SCS surface. According to previous studies, the pHpzc values of coconut leaves and mango peels were 3.2 and 4.6, respectively, and were reported to be low after sulfonation with H2SO4 [26, 27].

#### 3.1.3. FT-IR spectra

MB is a cationic molecule containing 6 carbon aromatic rings, nitrogen and sulfur in its molecular structure that affects the interaction of the adsorbent with the carbon surface [22]. The process of adsorption of MB to carbon occurs through electrostatic interactions, formation of hydrogen bridges, electron donor acceptor relationships, and the electron dispersing force of π-π between functional groups on the carbon surface with MB molecules [5]. Therefore, in addition to the surface area and porosity of the carbon adsorbent, the presence of functional groups such as −C=O, −COC-, −OH, −NH2, −C=S, −C=N and −S=O on the carbon surface plays an important role in increasing the adsorption capacity to separate MB [1, 9].
FT-IT results of SCS were bonded OH-group (3,000–3,500 cm−1), CH stretching (2,900–2,800 cm−1), C=O cabonyl groups (1,740–1,680 cm−1), and carboxylic groups (1,670–1,640 cm−1), CO stretch (1,450–1,300 cm−1), C-O-C groups (1,200–1,230 cm−1), SO3H (1,150–1,165 cm−1) and S=O groups (1,010–1,040 cm−1) peaks which appeared due to sulfonation (Fig. 2). In particular, the peak of 1,010–1,200 cm−1 increased significantly due to the introduction of sulfone groups. In addition, it was confirmed that the ether of 1,109 cm−1, the absorption peak of R-SO3H of 1,232 cm−1, and ketone peaks of 1,642 cm−1 and 1,477 cm−1 were sulfonated. In particular, the peaks of N-containing bioligands, R-SO3H absorption peak, carboxylic groups and bonded OH-group were larger than that of CS, and there were more functional groups. This indicates that SCS has a structure that is easier to adsorb MB ions than CS. Osman et al. [28] reported that the adsorption capacity of metals is proportional to the number of functional groups in the adsorbent. It is believed that the change of functional groups through sulfonation will affect the adsorption

### 3.2. Parametric Study

Development of an environmentally friendly adsorbent capable of adsorbing a large amount of harmful substances inexpensively and in a small amount is advantageous in terms of economy, but is also required in terms of environment. To determine the effect of the amount of SCS on the adsorption efficiency of MB, experiments were performed the concentration of MB was increased from 0.1 g/L to 1 g/L, around pH 7 and 25°C. The relationship between the MB removal efficiency of more than 90% and the amount of SCS is shown in Fig. S2, the correlation was 0.9982. As a result of calculating the amount of SCS required for MB removal with the correlation coefficient, the amount of about 19.5 mg of dye/g of SCS could be removed. When MB was removed using SCS, it is very economical because it uses lignocellulose derived agricultural by-products, which are discared wastes, so that the discarded resources can be reused. According to previous studies, when the adsorbent was sulfonated, the ion exchange capacity increased compared to the unmodified adsorbent, and accordingly, the removal efficiency of MB was improved [27, 29]. This is consistent with the research results of many researchers who adsorbed heavy metals in aqueous solutions by modifying agricultural waste as already mentioned in the introduction.

#### 3.2.2. Effect of pH

In order to examine the MB adsorption rate of SCS, adsorption kinetics were analyzed using pseudo-first order and pseudo-second order. Pseudo-first order depends on the concentration of only one reactant, that is, the monomolecular reaction [30]. Different reactants may be present in the aqueous solution, but each will be in zero order. Rodrigues and Silva [31] reported that the pseudo-first order of lagergreen is simple but theroretically inconsistent. Pseudo-second order depends on the concentration of one secondary reactant or two primary reactants [4]. Therefore, when analyzing the adsorption rate of various adsorbents in aqueous solution, it is often more suitable for pseudo-second order than pseudo-first order. The analysis results of adsorption kinetics are shown in Table 2 and Fig. S3. The correlation coefficient (R2) of the kinetic model was measured higher in pseudo-2nd-order (0.9775) than pseudo-1st-order (0.7814). Beside the qcal calculated in the pseudo-2nd-order model was closer to the measured qexp compared to the value calculated in the pseudo-1st-order model. Moreover, the value of χ2 in pseudo-2nd-order was lower (1.7231) than pseudo-1st-order (5.5846). Therefore, removal of MB from aqueous solution using SCS was more suitable for pseudo-2nd-order model than pseudo-1st-order.
Fig. S3(c) was applied to the internal particle diffusion model equation, and it was found that the data did not show a linear relationship and did not cross the origin. These results suggest that the process of adsorption of MB onto the SCS occurs through a complex mechanism through transfer of external substances and diffusion of internal particles [30]. Therefore, in the Fig. S3(c), mass transfer occurs in the initial area of adsorption (t1/2 < 1.7), and the adsorption process occurs due to diffusion of internal particles in the linear area after that (t1/2 > 1.7). The internal particle diffusion rate constant of MB obtained from the slope of the linear equation was 48.55 mg/g·h0.5.

#### 3.3.2. Isotherm modelling

An isothermal adsorption experiment was performed to obtain information on the adsorption characteristics of MB on SCS, and the obtained results are analyzed and summarized in Table 2. In general, isothermal adsorption is analyzed using models of Langmuir, Freundlich and Temkin. The Langmuir isothermal adsorption equation is a model that assumes that each reaction site has a uniform reaction intensity [25, 28]. The Freundlich equation is an adsorption model under the assumption that the adsorption site of the adsorbent is not uniform and the adsorption energy continuously decreases as the adsorption amount increases [32]. The Temkin isotherm indicates that the heat of adsorption of MB molecules decreases linearly rather than logarithmically with coverage [34]. A linear plot of Langmuir, Freundlich and Temkin are in Fig. S4.
The value of KF, which is a measure of the adsorption capacity calculated from the Freundlich equation, indicates that the higher the value, the better the adsorption capacity. In this experiment, 1/n was analyzed to be 0.132 and the KF value was high, indicating that the adsorption of MB onto SCS occurs easily in aqueous solution and adsorption capacity was excellent. The applicability of the adsorption model was that Langmuir’s correlation coefficient (R2 = 0.9833) was higher than Freundlich’s (R2 = 0.8722) or Temkin’s (R2 = 0.8685), so the adsorption of MB onto SCS was considered to be more suitable for the Langmuir model.
Table 3 compares the maximum adsorption amount of MB using lignin or ligno-cellulose or cellulose-based agricultural by-products. Overall, the modified adsorbent had a higher maximum adsorption amount than the unmodified natural adsorbent, which provided a good reason to modify the adsorbent. The maximum adsorption amount of MB using SCS was 504.3 mg/g, which was appropriately high compared to other adsorbents.

SCS is a strong acid cation resin (SAC). According to the literature, SAC resin adsorbs almost all cations contained in the aqueous solution and exchanges them for hydrogen ions [39]. Since this ion exchange process is reversible, when the ion exchange capacity is exhausted, the resin can be regenerated using a strong acid. In addition, since the SAC resin is well applied in all pH ranges, its application range is very wide [5]. Adsorption of MB in aqueous solution is highly dependent on the various polar functional groups on the surface [37].
According to FT-IR analysis, on the SCS surface through the sulfonation process, −SO3 groups were formed, which were concentrated with hydroxyl, carboxyl and carbonyl. Accordingly, depending on the functional groups available on the SCS surface, the adsorption mechanism of MB can be activated for various interactions. For example, electrostatic attraction between positively charged MB ions in aqueous solution and negatively charged functional groups on the SCS surface, and hydrogen bonding interactions between the surface hydrogen bonds of functional groups available on the SCS surface and the atoms of MB (Fig. 4).
In addition, according to the analysis of FT-IR, SCS has a structure that can be easily adsorbed to cations. The possible binding of the functional group to the MB on the surface of the SCS would be as follows.
##### (4)
$SCS-OH+C6H18N3SCl→SC-O-C6H18N3S+H+Cl-$
##### (5)
$SCS-COOH+C6H18N3SCl→SCS-COO-C6H18N3S+H+Cl-$
##### (6)
$SCS-SO3H+C6H18N3SCI→SCS-SO3-C6H18N3S+H+Cl-$

### 3.5. Thermodynamic Interpretation

In the adsorption process, the reaction temperature affects all potential ion exchange materials as well as the solubility products of metal ions, which can determine the rate of adsorption [4]. The solubility of metal ions affects adsorption efficiency because it may induce ion exchange between the metal ions contained in the aqueous solution and the surface of the adsorbent [27]. The effect of temperature on adsorption efficiency in aqueous solution was investigated, and the results are shown in Table 4 and Fig. S5. According to thermodynamic analysis, adsorption of MB onto SCS in aqueous solution was a spontaneous process, endothermic reaction and corresponds to a physical process.

### 4. Conclusions

This study attempted to remove the cationic dye MB from aqueous solution by SCS. After sulfonation of CS, the R-SO3H absorption peak, carboxylic groups and OH-group peaks were large on the surface of the adsorbent, and the surface area, pore diameter and ion exchange capacity were remarkably increased. As a result of adsorption kinetics and isothermal adsorption experiments, adsorption of MB to SCS was suitable for pseudo-2nd-order and Langmuir, and the maximum adsorption capacity of Langmuir was 504.3 mg/g. Finally, the adsorption of MB to the SCS was an endothermic reaction, and the adsorption efficiency improved as the temperature increased, and it was closer to physical adsorption than chemical adsorption. SCS showed excellent adsorption capacity of MB in aqueous solution. However, the powder of SCS is suitable for batch-testing, but it is considered that proper encapsulation is necessary for the convenience of use and prevention of mass loss in order to be applied to the field.

### Acknowledgment

This study was supported by the National Research Foundation of Korea(NRF) grant funded by the Korea government (MSIT) (No.2021R111A3059243)

### Notes

Author Contributions

H.J.C. (Prof. Ph.D) performed conceptualization, methodology, data curation, writing - original draft, visualization, investigation, software, validation, writing review & editing.

### References

1. Choi HJ, Yu SW. Biosorption of methylene blue from aqueous solution by agricultural bioadsorbent corncob. Environ Eng Res. 2019;24(1)99–106.

2. Li Y, Xiao H, Pan Y, Wang L. Novel composite adsorbent consisting of dissolved cellulose fiber/microfibrillated cellulose for dyr removal from aqueous solution. ACS Sustain Chem Eng. 2018;6:6994–7002.

3. Kumari S, Chauhan GS, Ahn JH. Novel cellulose nanowhiskers-based polyurethane foam for rapid and persistent removal of methylene blue from its aqueous solutions. Chem Eng J. 2016;304:728–736.

4. Dai Y, Sun Q, Wang W, et al. Utilization of agricultural waste as adsorbent for the removal of contminants: A review. Chemosphere. 2018;211:235–253.

5. Santoso E, Ediati R, Kusumawati Y, Bahruji H, Sulistiono DO, Prasetyoko D. Review on recent advances of carbon based adsorbent for methylene blue removal from waste water. Mater Today Chem. 2020;16:100233

6. Aruna , Bagotia N, Sharma AK, Kumar S. A review on modified sugarcane bagasse biosorbent for removal of dyes. Chemosphere. 2021;268:129309

7. Manna S, Roy D, Saha P, Gopakumar D, Thomas S. Rapid methylene blue adsorption using modified lignocellulosic materials. Process Saf Environ Process. 2017;107:346–356.

8. Jawad AH, Razuan R, Appaturi JN, Wilson LD. Adsorption and mechanism study for methylene blue dye removal with carbonized watermelon (Citrullus lanatus) rind prepared via one-step liquid phase H2SO4 activation. Surf Interfaces. 2019;16:76–84.

9. Zhang J, Koubaa A, Xing D, et al. Conversion of lignocellulose into biochar and furfural through boron complexation and esterification reactions. Bioresour Technol. 2020;312:123586

10. Jawad AH, Rashid RA, Ishak MAM, Wilson LD. Adsorption of methylene blue onto activated carbon developed from biomass waste by H2SO4 activation: kinetic, equilibrium and thermodynamic studies. Desalin Water Treat. 2016;57:25194–25206.

11. Zhu S, Xu J, Kuang Y, et al. Lignin-derived sulfonated porous carbon from cornstalk for efficient and selective removal of cationic dyes. Ind Crop Prod. 2021;159:113071

12. Roy R, Sajjadur Rahman MD, Raynie DE. Recent advances of greener pretreatment technologies of lignocellulose. Current Res Green Sustain Chem. 2020;3:100035

13. Supanchaiyamat N, Jetsrisuparb K, Knijneburg JTN, Tsang DCW, Hunt AJ. Lignin materials for adsorption: current trend, perspectives and opportunities. Bioresour Technol. 2019;272:570–581.

14. Li X, Lu X, Liang M, et al. Conversion of waste lignocellulose to furfural using sulfonated carbon microspheres as catalyst. Waste Manag. 2020;108:119–126.

15. Elangovan R, Philip L, Chandraraj K. Biosorption of chromium species by aquatic weeds: kinetics and mechanism studies. J Hazard Mater. 2018;152:100–112.

16. Choi HJ. Assessment of the adsorption kinetics, equilibrium, and thermodynamic for Pb(II) removal using a low-cost hybrid biowaste adsorbent, eggshell/coffee ground/sericite. Water Environ Res. 2019;91:1600–1612.

17. Hagesteijn KFL, Jiang S, Ladewig BP. A review of the synthesis and characterization of anion exchange membranes. J Mater Sci. 2018;53:11131–11150.

18. Barylak M, Cendrowski K, Mijowska E. Application of carbonized metal-organic framework as efficient adsorbent of cationic dye. Ind Eng Chem Res. 2018;57:4867–4879.

19. Furtmair M, Timm J, Marschall R. Sulfonation of porous materials and their proton conductivity. Micropor Mesopor Mat. 2021;312:110745

20. Dora S, Bhaskar T, Singh R, Naik DV, Adhikari DK. Effective catalytic conversion of cellulose into high yields of methyl glucosides over sulfonated carbon based catalyst. Bioresour Technol. 2012;120:318–321.

21. Feng Q, Cheng H, Chen F, Zhou X, Wang P, Xie Y. Investigation of cationic dye adsorption from water onto acetic acid lignin. J Wood Chem Technol. 2015;36:173–181.

22. Sabar S, Abdul Aziz H, Yusof NH, et al. Preparation of sulfonated chitosan for enhanced adsorption of methylene blue from aqueous solution. React Funct Polym. 2020;151:104584

23. Boota R, Bhatti HN, Hanif MA. Removal of Cu(II) and Zn(II) using lignocellulosic fiber derived from Citrus reticulata (Kinnow) waste biomass. Sep Purif Technol. 2009;44:4000–4022.

24. Benadjemia M, Millière L, Reinert L, Benderdouche N, Duclaux L. Preparation, characterization and methylene blue adsorption of phosphoric acid activated carbons from globe artichoke leaves. Fuel Process Technol. 2011;92:1203–1212.

25. Choi HJ. Assessment of the adsorption kinetics, equilibrium and thermodynamic for Pb(II) removal using a hybrid adsorbent, eggshell and sericite, in aqueous solution. Water Sci Technol. 2019;79(10)1922–1933.

26. Jawad AH, Mamat NFH, Abdullah MF, Ismail K. Adsorption of methylene blue onto acid-treated mango peels: kinetic, equilibrium and thermodynamic. Desalin Water Treat. 2017;59:210–219.

27. Li J, Li H, Yuan Z, et al. Role of sulfonation in lignin-based material for adsorption removal of cationic dyes. Int J Biol Macromol. 2019;135:1171–1181.

28. Osman HE, Badwy RK, Ahmad HK. Usage of some agricultural by-products in the removal of some heavy metals from industrial wastewater. J Phytol Res. 2010;2:51–62.

29. Weijue GAO, Inwood JPW, Fatehi P. Sulfonation of hydroxy methylated lignin and its application. J Bioresour Bioprod. 2019;4(2)80–88.

30. Lee SY, Choi HJ. Persimmon leaf bio-waste for adsorptive removal of heavy metals from aqueous solution. J Environ Manage. 2018;209:382–392.

31. Rodrigues AE, Silva CM. What’s wrong with lagergreen pseudo first order model for adsorption kinetics? Chem Eng J. 2016;306:1138–1142.

32. Yu SW, Choi HJ. Application of hybrid bead, persimmon leaf and chitosan for the treatment of aqueous solution contaminated with toxic heavy metal ions. Water Sci Technol. 2018;78(4)837–847.

33. Choi HJ, Yu SW, Kim KH. Efficient use of Mg-modified zeolite in the treatment of aqueous solution contaminated with heavy metal toxic ions. J Taiwan Inst Chem Eng. 2016;63:482–489.

34. Ma J, Yu F, Zhou L, et al. Enhanced adsorptive removal of methyl orange and methylene blue from aqueous solution by alkali-activated multiwalled carbon nanotubes. ACS Appl Mater Interfaces. 2012;4:5749–5760.

35. Yang J, Qiu K. Preparation of activated carbons from walnut shells via vacuum chemical activation and their application for methylene blue removal. Chem Eng J. 2010;165:209–217.

36. Salazar-Rabage JJ, Leyva-Ramos R, Rivera-Utrilla J, Ocampo-Perez R, Cerino-Cordova FJ. Biosorption mechanism of methylene blue from aqueous solution onto white pine (Pinus durangensis) sawdust: Effect of operating conditions. Sustain Environ Res. 2017;7:32–40.

37. Zhang S, Wang Z, Zhang Y, Pan H, Tao L. Adsorption of methylene blue on organosolv lignin from rice straw. Procedia Environ Sci. 2016;31:3–11.

38. Uddin MT, Islam MA, Mahmud S, Rukanuzzaman M. Adsorptive removal of methylene blue by tea waste. J Hazard Mater. 2009;164:53–60.

39. Ämmälä A, Laitinen O, Sirviö JA, Liimatainen H. Key role of mild sulfonation of pine sawdust in the production of lignin containing microfibrillated cellulose by ultrafine wet grinding. Ind Crop Prod. 2019;140:111664

40. Heidarinejad Z, Rahmanian O, Fazlzadeh M, Heidari M. Enhancement of methylene blue adsorption onto activated carbon prepared from data press cake by low frequency ultrsound. J Mol Liq. 2018;264:591–599.

41. Reffas A, Bernardet V, David B, et al. Carbons prepared from coffee grounds by H3PO4 activation: characterization and adsorption of methylene blue and Nylosan Red N-2RBL. J Hazard Mater. 2010;175:779–788.

42. Robati D, Bagheriyan S, Rajabi M, Moradi O, Ahmadi Peyghan A. Effect of electrostatic interaction on the methylene blue and methyl orange adsorption by the pristine and functionalized carbon nanotubes. Physica E. 2010;83:1–6.

43. Que W, Jiang L, Wang C, et al. Influence of sodium dodecyl sulfate coating on adsorption of methylene blue by biochar from aqueous solution. J Environ Sci. 2018;70:166–174.

44. Lasheen MR, Ammar NS, Ibrahim HS. Adsorption/desorption of Cd(II), Cu(II) and Pb(II) using chemically modified orange peel: equilibrium and kinetic studies. Solid State Sci. 2012;14:202–210.

##### Fig. 1
pHpzc of SCS suspensions in aqueous solution at ambient conditions.
##### Fig. 2
A FT-IR spectra of CS and SCS.
##### Fig. 3
Effect of pH on the adsorption of MB (SCS: 1 g/L, MB concentration: 10 mg/L, agitation: 120 rpm, T: 25°C).
##### Fig. 4
Possible adsorption mechanism of ligno-cellulose derived SCS with sulfonation.
##### Table 1
Characteristic of CS and SCS (unit: %)
Component (mass %) CS SCS
O 36.23 52.48
C 55.42 41.24
H 2.33 5.76
N 1.53 1.61
S - 1.32
Mg 0.09 0.10
Surface property
Pore volume (cm3/g) 0.102 0.164
Pore diameter (nm) < 2 nm 95.4
2–30 nm 4.6 96.8
> 30 nm - 3.2
BET surface area (m2/g) 8.32 24.23
Ion exchange capacity (meq/g) 1.63 4.13
##### Table 2
Kinetics and Isothermal Parameters for the Adsorption of MB onto SCS
Kinetic model Pseudo-first-order [ln(qe-qt) = lnqe-k1t] Pseudo-second-order [ $tqt=1k2qe2+tqe$] Intraparticle diffusion [qt = kd t1/2 + C]

qexp k1 qe,cal χ2 R2 k2 × 10−3 qe.cal χ2 R2 Kd C χ2 R2
497.6 0.219 356.5 5.5846 0.7814 6.42 413.2 1.7231 0.9775 53.56 195.76 3.6521 0.8176

Isotherm Parameters Values
Langmuir [ $Ceqe=1qmaxkL+1qmaxCe$] qm (mg/g) 504.3
KL (L/mg) 0.23

χ2 1.5026
R2 0.9833

Freundlich [ $lnqe=lnkF+1nlnCe$n] KF ((mg/g) (L/mg)1/n) 123.67
1/n 0.132
χ2 5.2062
R2 0.8722

Temkin[ln qe = B lnkT + B lnCe] B (J/mol) 18.06
KT (L/mg) 56.32
χ2 11.5932
R2 0.8685

[i] qe: adsorbed amount of MB at equilibrium (mg/g), qt: amounts of MB adsorbed by SCS at equilibrium time t (mg/g), k1: Pseudo-1st-order constant (1/min), k2: Pseudo-2nd-order constant (g/mg·min), t: time (min), kd: rate constant of intraparticle diffusion kinetic (mg/g·h0.5), C: constant associated with the boundary layer thickness. Ce: MB concentration at equilibrium (mg/L), qmax: Langmuir maximum adsorption capacity (mg/g), KL: Langmuir constant (L/mg), KF: adsorption capacity (mg/g)(L/mg)1/n, 1/n: adsorption intensity of the system, kT: Temkin isotherm constant (L/mg), B: correlated to adsorption heat

##### Table 3
Comparison of the Maximum Adsorption Capacities of MB Dye onto Agricultural Waste Adsorbents
Walnut shell 315.0 [35]
White pine sawdust 102.0 [36]
Rice straw 40.0 [37]
Tea waste 85.2 [38]
sulfonated lignin-based hydrogels 540.5 [27]
lignin derived sulfonated porous carbon 420.4 [12]
Carbonylated cellulose/ microfibrillated cellulose spheres 303.0 [2]
Cellulose nanowhiskers based polyurethane foam 554.8 [3]
Activated carbon nanotubes 399.0 [34]
Acetic acid lignin 63.3 [21]
sulfonated chitosan 351.7 [22]
sulfonated corn stalk 504.3 This study
##### Table 4
Thermodynamic Parameters for Adsorption of MB onto SCS
Temperature (K) Thermodynamic [ΔG0 = ΔH0–TΔS0]

ΔG° (kJ/mol) ΔH (kJ/mol) ΔS (J/mol·K)
298 −12.78 12.36 428.74
303 −12.99
313 −13.42
323 −13.85
TOOLS
Full text via DOI
Supplement
E-Mail
Print
Share:
METRICS
 2 Crossref
 0 Scopus
 1,161 View